6HOMOGENEOUS NUCLEATION The classical theory of nucleation assumes that clusters are formed in solution by an addition mechanism:A + A A2A2 + A A3A3 + A A4An-1 + A An (critical cluster)that continues until a critical size is reached(n = tens to thousands)
7CLASSICAL THEORY OF NECLEATION The overall excess free energy, G, between a small solid particle of solute (assumed to be a sphere of radius r) and the solute in the solution is defined as:(1)whereGS : surface excess free energy, i.e. the excess free energy between the surface of the particles and the bulk of the particle)GV : volume excess free energy, i.e. the excess free energy between a very large particle, r = , and the solute in solution.
8GS is a positive quantity and is proportional to r2 GS is a positive quantity and is proportional to r2. In a supersaturated solution GV is a negative quantity and is proportional to r3.(2)whereGv : free energy change of the transformation per unit volume (a negative quantity) : surface energy, i.e. interfacial tension between the developing crystalline surface and the supersaturated solution in which it is locatedThe two terms on the right-hand side of eq. (2) are of opposite sign and depend differently on r, so G passes through a maximum.
9This maximum value, Gcrit, corresponds to the critical nucleus, rc This maximum value, Gcrit, corresponds to the critical nucleus, rc. For spherical cluster, it is obtained my maximizing eq. (2), setting d(G)/dr = 0:(3)Where Gv is a negative quantity. From eqs. (2) and (3):(4)Particles smaller than rc will dissolve, or evaporate if the particle is a liquid in a supersaturated vapor, because only in this way can the particle achieve a reduction in its free energy. Similarly, particles larger than rc will continue to grow.
11The rate of nucleation, B0, e. g The rate of nucleation, B0, e.g. the number of nuclei formed per unit time per unit volume, can be expressed in the form of the Arrhenius type of expression:(5)wherek : Boltzmann constant = J K-1A : pre-exponential factor(theoretical value = 1030 nuclei/cm3 s)The basic Gibbs-Thomson relationship for a non-electrolyte:(6)whereS : supersaturation ratio = c/c*v : molecular volume
12From eq. (6):Introducing the above equation into eq. (3) gives:(7)Introducing eq. (7) into eq. (4) gives:(8)And from eq. (5) gives:(9)
13Induction Time for Nucleation of Water Vapor SInduction time1.02.01062 years3.0103 years4.00.1 seconds5.010-13 secondsIn the case of nucleation of water vapor, a ‘critical’ super-saturation could be said to exist in the region of S ~ 4.0, but it is also clear that nucleation would have occurred at any value of S > 1 if sufficient time had been allowed to elapse.
14Effect of supersaturation on the nucleation rate
15The rate equation predicts exponential growth once a critical supersaturation is attained. In practice, an optimal temperature exists below which the liquid is too viscous to nucleate and above which molecular motions prevent crystal formation.The viscous effects can be incorporated into the rate equation by taking into account the viscous free energy(10)This was observed by Tamman (1925) for several organic salts, and Mullin and Leci (1969) for the spontaneous nucleation of citric acid solutions and is shown in the following figure.
16Spontaneous nucleation in supercooled citric acid solution: (A) 4.6 kg of citric acid monohydrate/kg of "free" water (T= 62 °C) and (B) 7.0 kg/kg (T= 85 °C).
17An empirical approach to the nucleation process is described by Nielsen (1964), expressing a relationship between the induction period, tind (the time interval between mixing two reacting solutions and the appearance of crystals) and the initial concentration, c, of the supersaturation solution:(11)where k : constantp : number of molecules in a critical nucleus
18HETEROGENEOUS NUCLEATION A foreign substance present in a supersaturated solution is generally known to reduce the energy required for nucleation.Nucleation in a heterogeneous system generally occurs at a lower supersaturation than a homogeneous system.Partial attraction is possible in a case where the foreign substance and the crystal have almost identical atomic arrangement.It was shown (Preckshot and Brown 1952) that the energy for nucleus formation was reduced only if the difference in iso- morphism between the crystal and the foreign particle was <15%.For differences >15%, the energy requirements were similar to that for a homogeneous system.
19SECONDARY NUCLEATIONSecondary nucleation results from the presence of crystals in the supersaturated solution.These parent crystals have a catalyzing effect on the nucleation phenomena, and thus, nucleation occurs at a lower supersaturation than needed for spontaneous nucleation.Although several investigations of secondary nucleation exist, the mechanisms and kinetics are poorly understood.
20Strickland-Constable (1968) described several possible mechanisms of secondary nucleation: ‘Initial’ breeding (crystalline dust swept off a newly introduced seed crystal)‘Needle’ breeding (the detachment of weak out-growths)‘Polycrystalline’ breeding (the fragmentation of weak polycrystalline mass)‘Collision attrition’ breeding (a complex process resulting from the interaction of crystals with one another or with parts of the crystalline vessel)
21Factors Affecting Secondary NucleatiON Several factors influence these processes:the supersaturation,the rate of cooling,the degree of agitation, andthe presence of impurities.
22SupersaturationThe degree of supersaturation is the critical parameter controlling the rate of nucleation.The size of the critical nucleus decreases with increasing supersaturation, thus, the probability of the nuclei surviving to form crystals is higher.In general, nucleation rates are enhanced with increasing supersaturation. However, the nucleation exponent is found to be lower than that for primary nucleation
23TemperatureThe role of temperature in the production of secondary nuclei is not fully understood.For several systems, the nucleation rate declined with increasing temperature for a given supersaturation.A few contradictory results exist - Genck and Larson (1972) found a decrease in nucleation rate with increasing temperature for a potassium nitrate system and increasing rates with increasing temperature for a potassium chloride system.It was shown by Nyvlt (1981) and others that the nucleation order is not sensitive to temperature variations.
24Stirring Stirring the solution leads to lower nucleation rates. However, Sikdar and Randolph (1976) found that the nucleation rate increased with the degree of agitation for smaller crystals of magnesium sulfate (8-10 m) — the nucleation rates were independent of the degree of agitation for larger crystals.The results of Melia and Moffit (1964a, 1964b) on the secondary nucleation of potassium chloride are shown in the following figure; they found that the nucleation rate increases with supersaturation, and the degree of supercooling and agitation
25Dependence of number of secondary nuclei produced on stirrer speed and supercooling in secondary nucleation of potassium chloride
26Hardness of the contact material In general, it was found that a harder material is more effective in enhancing the nucleation rates.For example, it was found that a polyethylene stirrer reduced the nucleation rates by a factor of 4-10, depending on the agitationCrystal hardness also affects nucleation behavior — a hard, smooth crystal is less effective.Irregular crystals with some roughness are generally more active.
27Effect of agitator speed on secondary nucleation rate for steel and plastic impellers.
28ImpurityIt is well known that a small amount of impurity can profoundly affect the nucleation rate, however, it is impossible to predict the effect prior.The presence of additives can either enhance or inhibit the solubility of a substance.Enhanced solubilities would lead to lower supersaturations and lower growth rates.The effect of impurities is complex and unpredictable.
29NUCLEATION KINETICSA general theory for the prediction of nucleation rates does not exist.Several correlations based on the power law model have been found to explain most of the experimental data satisfactorily.The power law is given by:(no/m3.s)(12)This form is valid if the adsorption layer mechanism is the source of nuclei.The nucleation rate in this case is independent of the suspension concentration.
30In the industrial crystallizer, most of the nuclei are generated by contact with the crystallizer environment.The nucleation rate in this case is a function of the degree of agitation, the suspension density, and the supersaturation.(13)where W : agitation rate (rpm)MT : suspension density (mass of crystals per volume of solution).In some situations an equation that does not include the effect of agitation is used(14)In this case may vary with the agitation rate.
31The kinetics for secondary nucleation can be measured either by measuring the width of the metastable zone, the induction time, or by counting the number of nuclei formed.One of the methods for the determination of nucleation rates is by measuring the maximum possible supercooling that can be obtained in a saturated solution when it is cooled at different rates (metastable zone width measurement).The polythermal experiment (proposed by Nyvlt 1968) is carried out in a jacketed crystallizer cooled by a circulating water/ethylene-glycol bath accurate to ± 0.1 °C.The temperature can be increased or decreased at a constant rate by a programmed controller.The crystallizer is fitted with an accurate thermometer ±0.1 °C to read the solution temperatures.A schematic of the apparatus is shown in the following figure.
32Schematic diagram of apparatus for measurement of nucleation rates.
33Approximately 200 ml of saturated solution is placed in a crystallizer and allowed to equilibrate thermally.The solution is stirred at a constant rate and cooled slowly until a number of small crystals are formed.The temperature of the solution is then raised at a very slow rate until the last crystal disappears.This temperature is denoted as the saturation temperature, Ts.The solution is then heated to a temperature 1° above Ts and maintained for 30 min.The solution is now cooled at a constant rate (r1) and the temperature at which the first crystal appears is noted (T1).The difference between this temperature and the saturation temperature is denoted as AT1max for the cooling rate r1.The experiment is repeated for two different cooling rates.
34CRYSTAL GROWTHThe growth of a crystal is often described by the change in some dimension of the crystal with time linear growth rate .However, crystals are made up of a number of faces that can grow at different rates.Therefore, a fundamental expression of the growth rate is the linear growth rate of a particular face.This refers to the rate of growth of the face in the direction normal to the face.
35When a linear growth rate is used to describe the growth of an entire crystal it is describing the increase in some characteristic dimension of the crystal.If the crystal was a sphere, the characteristic dimension would be the diameter and we would express the crystal growth rate by the increase of the diameter with time.If the crystal is of another shape, the characteristic dimension used is usually the second longest dimension.This can be understood by thinking of what happens when you pass crystals through screens or sieves. The dimension of the crystal, which determines if it will pass through a sieve of a given size, is the second largest dimension rather than the largest dimension.This characteristic dimension can be related to the volume and surface area of the crystal through the shape factor.
36Another way of measuring crystal growth rates is through the measurement of the mass change of the crystal.The increase in mass with time is often used and can be directly related to the overall linear growth velocity through the relation(1)whereRG : increase of mass per unit time per unit surface areaA : surface area of the crystal, : volume and area shape factors, respectively : crystal densityL : characteristic dimension
37THEORIES OF CRYSTAL GROWTH Surface structure of a growing crystal
38From an energetic point of view, C is more favorable than B, and B more favorable than A. This can be generalized by saying that molecules tend to bond at locations where they have the maximum number of nearest neighbors. These are the most energetically favorable sites.The general mechanism for incorporation of a molecule into a crystal face is its adsorption onto the surface followed by its diffusion along the surface to a step (B-type) or kink (C-type) site for incorporation.From this explanation you can see why crystals grow in a layer-by-layer fashion since it is easier for molecules to bond to an existing step that is spreading over a surface than to form a new one.
39Formation of two-dimensional critical nucleus on a crystal surface Two-Dimensional Growth TheoriesMolecules will be continuallyabsorbing on the surface diffusing and desorbing. They also will collide with each other and form two-dimensional aggregatesFormation of two-dimensional critical nucleus on a crystal surface
40Burton-Cabrera-Frank (BCF) Model Development of a growth spiral from a screw dislocation
42CRYSTAL GROWTH KINETICS The relationship between supersaturation and crystal growth:(length/time) (1)and(mass/time) (2)The power g in the growth equations does not depend on theform of the equation used and is normally a number between 1 and 2
43The constants in eqs. (1) and (2) can be related to each other through the expression: (3)The constants kg and Kg are temperature-dependent and areusually fit to the Arrhenius equation to obtain a general expression for growth rate as a function of temperature.(4)whereA : pre-exponential factorEG : activation energy
44Measurement of Crystal Growth Rates 500 – 1000 cm32.5 cm diameterRecirculation apparatus for single crystal growth
46Effect of flow rate on the growth rate of single crystal of potassium aluminum sulfate to dodecahydrate
47The methods for measurement of crystal growth kinetics discussed to this point all involve the growth of a single seed crystal.This is clearly different from the environment in an industrial crystallizer where many crystals are growing in a suspension.A laboratory method known as a fluidized bed crystallizer, which attempts to measure the growth rates of a number of crystals, is shown in the following figure.
49In this method, solution is circulated through a crystallizer in which seed crystals are suspended by the flowing fluid.The flow is such that the crystal will not settle and will not flow out of the crystallization vessel.As in single crystal growth experiments, the mass of solute depositing on the growing crystals must be small enough so that the system is considered to be at constant supersaturation.By using seed crystals of the same initial size, the final size and mass of the crystals can be used to obtain an average growth rate.The most common method for obtaining crystal growth kinetics involving suspensions involves the use of a mixed suspension, mixed product removal (MSMPR) continuous crystallizer operating at steady state.